1. INTRODUCTION The Non-Destructive Test (NDT) is defined as the application of different control methods that allow the examination of materials or constructions, without altering or affecting their future use. During their implementation the materials characteristics are not altered, nor are their physical and mechanical properties. NDT is valuable to high-risk constructions (airplanes, underwater pipes, offshore platforms, nuclear reactors, fuel tanks, ships), because it enables a continuous control. The offshore and shipbuilding industry is largely based on welded construction elements and extending to welders constructions. The welding quality is a crucial sufficient factor, evaluated through the welding quality test, and the reliable operation of any metallic shipbuilding construction. The quality test demands and more specifically «the damage tolerance» is differentiated where applicable (Fitness For Purpose), keeping in mind the techno-economic parameters of the welding technology. NDT is the basic tool for quality testing in the offshore industry. 3
2 NDT METHODS Until today many NDT methods have developed. For the choice of the correct method, the problem must be fully specified and to be aware of the basic operations of each method, in order to exploit its full potentials. Not all methods have the ability to effectively detect all the types of imperfections-faults. Subsequently, the most widely used NDT methods are reported to the material testing. 4
1 VISUAL INSPECTION Visual Inspection is a NDT Method, which provides the means for the control of surface imperfections- damages, such as corrosion, cracks and other surface discontinuities detected using the eye. Visual testing can be improved by using a wide variety of optical equipment, fiberscopes and boroscopes, also used for the NDT of inaccessible areas on the inner part of the construction. The boroscopes are devices that use a fiber optic system for the transfer of the image from the object being examined to the eyepiece system. 5
2 LIQUID PENETRANT INSPECTION Liquid penetrant inspection reveals surface flaws by the bleed-out of a penetrating medium against a contrasting background. The surface is sprayed with a liquid or a solid developer, capable of presenting the penetrant liquid that has penetrated to the imperfections. The resultant indications reveal the presence of the flaw so that it can be visually inspected and evaluated. For better results fluorescent liquids are used and the inspection is done under an ultraviolet (black) light. 6 The three stages of the penetrant liquid method.
3 MAGNETIC PARTICLE INSPECTION Magnetic particle inspection is a NDT and is used to locate surface and slight subsurface discontinuities or defects in ferromagnetic materials. At the points where there is a discontinuity the magnetic lines leave the surface of the material (Figure 1.3). This deviation, and consequently the existence of discontinuity, is seen with the application of ferromagnetic particles on the surface, either in the form of dust or particles in a liquid carrier (water, oil). The particles are drawn, at the areas where the deviation appears, and give the approximate size, the position and the shape of the discontinuity. 7
4 RADIOGRAPHIC METHODS Radiographic testing is a non-destructive inspection method based on using short wavelength electromagnetic or nuclear radiation passing through the material. The material under test is placed between the source of radiation and the surveying instrument. Materials with imperfections, areas of reduced thickness or lower material density allow more, and therefore absorb less, radiation which is tested. The differences, in the outbound radiation from the material, are recorded in a radiographic film or other means (Figure 1.4). With this way, you can identify imperfections (i.e.: cracks) and determine their size. 8
5 ACOUSTIC EMISSION The acoustic emissions are sound waves, of which are produced by the sudden charge or discharge of the materials, with mechanical or thermal loads. The sources of the acoustic emissions are plastic deformations of the materials, which are connected to mechanisms of defects evolution, such as crack propagation. When sudden relocations happen to these sources sound waves are produced which are spread to the whole construction and stimulate a piezoelectric head. The data are collected and followed by an analysis and processing. This method of acoustic emission detects the evolution of the imperfections-defects, in contrast to most methods of NDT, which detect the existence. 9
Levels of Inspection Three basic types or levels of inspection are used for inspecting marine facilities. The resources and preparation needed to do the work distinguish the level of inspection. Also, the level of inspection determines the type of damage/defect that is detectable : LEVEL I LEVEL II LEVEL III
Level I - General Visual Inspection. The Level I effort can confirm as-built structural plans and detect obvious major damage or deterioration due to overstress (collisions, ice), severe corrosion, or extensive biological growth and attack. The Level I will provide initial input for an inspection strategy. Although this is an overview, close attention should be given to confirming or providing information to update available facility drawings and condition evaluations. This type of inspection does not involve cleaning of any structural elements and can therefore be conducted much more rapidly than the other types of inspections. The Level I effort is essentially a general inspection swim-by overview. It does not involve cleaning of structural elements, which allows the inspection to be conducted rapidly. The underwater inspector relies primarily on visual and/or tactile observations (depending on water clarity) to make condition assessments. These observations are made over the specified exterior surface area of the underwater structure, whether it is a quay wall, bulkhead, seawall, pile, or mooring.
Level II - Close-Up Visual Inspection. Level II efforts are complete, detailed investigations of selected components or subcomponents, or critical areas of the structure, directed toward detecting and describing damaged or deteriorated areas that may be hidden by surface biofouling. Limited deterioration measurements are obtained. These data are sufficient for gross estimates of facility load capability. This type of inspection will generally involve prior or concurrent cleaning of part of the structural elements. Since cleaning is time consuming, it is generally restricted to areas that are critical or that may be typical of the entire structure. The amount and thoroughness of cleaning to be performed are governed by what is necessary to determine the general condition of the overall facility. Simple instruments such as calipers and measuring scales are commonly used to take physical measurements.
Level III - Highly Detailed Inspection. This level of inspection is primarily designed to provide data that can be used to perform a structural assessment and will often require the use of Nondestructive Testing (NDT) techniques. The procedures are conducted to detect hidden or imminent damage, loss in cross-sectional area, and material homogeneity. The training, cleaning, and testing requirements will vary depending on the type of damage/defect that is to be investigated and the type of inspection equipment to be used. A Level III examination will normally require prior cleaning. In some cases, Level III inspections will require the use of partially destructive techniques such as sample coring in wood or concrete, material sampling, and in-situ surface hardness.
The use of Level III inspection techniques is usually limited to key structural areas that may be suspect, or to structural areas that may be representative of the overall structure. Level III inspections will require considerably more experience and training than Level I or Level II inspections, and should be accomplished by qualified engineering or testing personnel. This type of inspection is covered by special rules and regulations
MO On steel H-piles, pipe piles, and sheet piles, metal thickness measurements are made with ultrasonic thickness equipment. In addition, electrical potential measurements, using a half-cell, are taken to verify the performance of the cathode protection system for steel structures. Concrete surfaces can be evaluated for hardness using a rebound hammer. Wood is inspected using calipers, ice picks, and hammers, and in some cases an incremental borer is used to obtain a core sample. However, depending upon visibility, marine growth, and extent of deterioration, this may be adjusted as the inspection proceeds. The underwater inspection may be accomplished by a qualified engineering diver or by a qualified, certified diver, supervised by an engineer. An experienced engineer skilled in inspection procedures and techniques must perform the structural assessment.
Capability of Each Level of Inspection For Detecting Damage to Waterfront Structures.
The time and effort required to carry out the three different levels of inspection are quite different. The time required for any particular level will depend on a number of factors, including 1.visibility, 2.currents, 3.wave action, 4.water depth, 5.severity of marine growth, 6. and the skill and experience of the diver.
Production Rate for Surface and Underwater Inspection of Structural Elements. Table provides a guide for estimating the time required to conduct Level I and Level II inspections. This information is based on: (1) A water depth of 30 to 40 feet (2) Visibility of 4 to 6 feet (3) Warm, calm water (4) Moderate marine growth (about 2 inches thick) (5) An experienced diver of average skill
Planning for Inspection Before starting a facility inspection, all available information about the facility should be obtained. This will usually require a preliminary visit to the facility. The Engineer in Charge should meet with the local staff engineer and obtain copies of the facility drawings and general background about the existing condition of the facility. Any unique features or special problems that may be encountered should be noted. Local information that should be obtained includes: Wave action Atmospheric temperature range Water temperature range Tidal range Water depths Water visibility Currents Any condition that could have a direct impact on the time needed to perform an inspection, such as amount of biofouling growth on piles or any other condition that would inhibit the performance of an inspection such as ice or seasonal flooding. Ship traffic and facility berthing requirements.
The bathymetric and oceanographic data, as well as information on nearby obstructions or activities, will accelerate the planning process and will aid in determining the levels of inspection to be used. The time and effort required to carry out the three different levels of inspection will vary considerably. The factors affecting the time required will include whether the inspection is surface or underwater; the environmental factors mentioned above; and the skill and experience of the inspector. Information about the local support, equipment, and utilities should be acquired prior to the inspection. Once the information about the facility has been collected, an inspection plan should be developed. The written plan should be like a statement of work containing a scope of work, specifying the sampling criteria. It should specify responsibilities, tasks, schedules, and equipment to be used.
Various zones of influence on piling Statistical software has been developed which identifies inspection frequencies based on cost when known or estimated structural data is inputted. The frequencies obtained will be unique to the facilitys situation. Inspection Frequency
Documentation of Inspection For the results of the inspection to be useful, they must be documented in a clear and concise manner and in accordance with generally understood terminology. Inspectors should maintain daily logs of inspection details including measurement data, locations of observation, and water depths, if relative. Inspection forms and reports should be completed as soon as possible after the inspection has been completed. Standard forms and report formats greatly facilitate the documentation procedure and are essential for comparing the results of the present inspection with past and future inspections. Steel pile inspection results are usually recorded in terms of remaining metal thickness. It should be noted, however, that the categorization of a defect, i.e., moderate, major, etc., will depend on the water depth. Piles in deeper water, with a long unsupported length, are susceptible to buckling, and loss in strength becomes more critical.
Example of a Standard Pile Inspection Report Form
Recording Tools. Recording tools and equipment are required to provide a complete documentation of the condition of the structure. Simple tools such as clipboards, forms, and video recorders for above water inspections, or a Plexiglas slate and grease pencil for underwater inspection, provide the basic documentation tools. More in-depth documentation may be obtained with above-water or underwater photography using colored still-frame cameras or colored video, or closed-circuit television. The latter may be very valuable in expediting major underwater inspections. For underwater inspections in turbid water, a clear-water box may be fitted to the lens of the photographic or video equipment to improve visibility between the lens and surface to be inspected.
STEEL STRUCTURES Types of Steel Structures In marine applications, steel (common steels for marine applications Grade A, B, D, E DS, CS) has many uses as a construction material. Steel piles, either H-piles or pipe piles, are used as support members for open piers, wharves, and other waterfront structures and facilities. Steel sheet piling is used primarily as a retaining wall structure for bulkheads used in the support of piers, wharves, dry-docks, and quay walls as well as near-water, earth- retaining structures. Fabricated structural steel members, whether tubular, plate, or other shapes, are used to construct undersea support towers for testing ranges, instrument arrays, and operation support platforms.
Deterioration of Steel Structures There are six major types and causes of steel structure deterioration in the marine environment: Corrosion Abrasion Loosening of structural connections Fatigue Overloading Loss of foundation material
Corrosion. Corrosion is the principal cause of deterioration of steel waterfront structures. Corrosion of steel is an electrochemical process that converts the steel into iron oxides. These iron oxides are easily recognized by their reddish-brown color and are commonly called rust. The rust may remain in place in the form of an encrustation or may naturally fall away or be removed by wave action or abrasion. The corroded surfaces are usually irregular and in some cases the attack in localized areas will be much greater than in other areas resulting in pitting. Over a period of time, unchecked corrosion will reduce the structural integrity of steel components of waterfront structures. On bare unprotected steel pilings, corrosion is often most severe just above the high tide line, with another zone of severe attack just below the low tide line.
Severe Corrosion, Just Above High Tide Line and Just Below Low Tide Line.
Galvanic corrosion occurs when two dissimilar metals are in electrical contact and both are submerged. Salt water is an excellent electrical conductor, and galvanic corrosion resulting from dissimilar metals in contact is a significant problem on waterfront structures. The possibility of galvanic corrosion must be considered whenever dissimilar metals are used in marine structures. An effect similar to galvanic corrosion can occur when there is a difference in environment between different areas on a single metal. When oxygen levels are limited, by reduced free access to freshly oxygenated water, in areas such as the threads of a bolt or between structural members, the difference in oxygen content can cause an electrical current to flow between the areas of high and low oxygen content. This effect is particularly severe on stainless steels and aluminum alloys. A difference in environment with resulting accelerated corrosion can also be created when a surface is partially covered by an electrically conductive material such as concrete. Corrosion can also be accelerated by the action of bacteria. In the absence of oxygen, sulfate-reducing bacteria can grow, and the sulfides they produce can cause rapid attack on steel. Finally, corrosion can be initiated by the presence of stray currents, e.g., from nearby electrical power lines.
Abrasion. Abrasion of steel structures can generally be recognized by a worn, smooth, polished appearance of the surface. Abrasion is caused by continual rubbing of adjacent moving steel surfaces, or by the exposure of structural components to wave action in areas of sandy bottom. Steel sheet piling and pile-supported structures are particularly susceptible to sand abrasion in exposed locations. Abrasion of steel structures is a problem because it removes both protective coatings and protective layers of corrosion products, thus accelerating corrosion.
Structural Connection Loosening. Structural connections joined together by rivets or bolts have a tendency to work loose over an extended period of time. Connection loosening can result from impact loading of the type imparted by a vessel striking a pier or wharf fender system. Wave action and reciprocating machinery mounted on or below pier or wharf decks are other sources of possible connection loosening. Corrosion of bolts, rivets, nuts, washers, and holes can also contribute to connection loosening. Loosening of connections will tend to produce misalignment in mating surfaces, which, in turn, can result in distortion and stress concentrations in framing members.
Fatigue Failure. Fatigue failure results in the fracture of structural members as a consequence of repeated high loading. Fatigue distress can be recognized by a series of small hairline fractures perpendicular to the line of stress in the member. Tubular connections of offshore platforms are particularly susceptible to fatigue failure. Fatigue cracks are difficult to locate. Since fatigue cracks represent an extremely dangerous condition in steel marine structures, extreme care must undertaken when inspecting structural members subjected to repetitive loading, particularly high wave loading.
Overloading. Steel structural elements are sensitive to impact damage from berthing vessels and other types of accidental overloading. Impact or collision damage can generally be recognized by the appearance of local distortion (deformation) of the damaged member. This damage is generally characterized by a sharp crimp or a warped surface.
Foundation Deterioration. Loss of foundation material from around steel piles leads to accelerated corrosion and loss of column strength of the piles. The loss of foundation material is usually caused by the scouring of material from around the piles. Scouring can be caused by an increase in the velocity of the water passing by the piles or a change in the currents direction. If the piles thus exposed are not protected, eventual collapse of the structure is possible. A loss of foundation material in front of a sheet pile bulkhead may cause kick-out of the toe of the wall and result in total failure.
Typical Inspection Procedure Surface Inspections. Generally, visual inspections will allow detection and documentation of most forms of deterioration of steel structures. In the event that more detailed NDT techniques may be required under a Level III inspection, a plan and sampling techniques need to be developed and tailored to the specific areas of concern. Some types of corrosion may not be detected by visual inspections. For example, inside steel pipe piling, anaerobic bacteria corrosion caused by sulfate-reducing bacteria is especially difficult to detect by visual inspection. Fatigue distress can be recognized by a series of small hairline fractures perpendicular to the line of stress but these are difficult to locate by visual inspection. This type of problem, however, is more prevalent to offshore platforms with welded structural connections than to standard piers and wharves. Cathodic protection systems need to be closely monitored both visually and electrically for signs of loss of anodes, wear of anodes, disconnected wires, damaged anode suspension systems, and/or low voltage.
Underwater Inspection. Underwater Inspection of a steel waterfront structure should proceed as outlined in Table.
Ultrasonic Inspection. Ultrasonic thickness measurement equipment is available for inspecting steel structures. Thickness measurements are obtained because certain types of ultrasonic waves travel at a constant speed through a material, because they travel in straight lines, and because a portion of the wave is reflected when it meets an interface. The difference in time between the detection of the front surface and back surface echoes is correlated to the thickness of the material. Ultrasonic thickness measurements require a thorough removal of marine growth and scale and can be unreliable if the surface on which the instrument is placed is heavily pitted. Adequate training and experience are required to obtain readings and to evaluate the measurements made with this equipment.
Under water UT measurements kit
Underwater Magnetic Particle Testing. Underwater magnetic particle testing (UWMT) is a nondestructive method for locating and defining surface discontinuities (such as cracks) in magnetic materials underwater. Its principle of operation is that magnetic particles are attracted to flux leakages at the surface of magnetized materials and form indications of discontinuities located either at or just below the surface. In operation, the magnetic material or item of interest is magnetized using an electromagnetic yoke specially designed for underwater use. Wherever surface discontinuities exist within the yokes field of influence, magnetic flux will leak from the surface of the part. A slurry of magnetic particles are attracted to, and aligned with, the leaking magnetic flux. The particles are brightly colored and form a visible indication corresponding to the location of discontinuities at or very near the parts surface.
UWMT Applications - Underwater magnetic particle testing is used primarily as a quality assurance tool to support underwater welding on ship structures. It can also be used to inspect hulls or other magnetic components for surface discontinuities such as cracks and lack of fusion in welds. UWMT can be used to define the true length (and locate the true ends) of discontinuities detected visually and to help determine where corrective measures (e.g., stop drilling) should be applied. UWMT Limitations (1) Underwater magnetic particle testing has limited subsurface capability. It is considered to be strictly a method for detecting and measuring surface discontinuities. It is not an approved method for detection of subsurface discontinuities. (2) The adequacy of inspection with UWMT (as with most nondestructive test methods) is largely a function of the operators knowledge and skill. Inspections with UWMT are to be performed only by personnel trained and specifically certified in UWMT. (3) UWMT is limited to ferromagnetic materials, which include most steels. For most applications, a simple check with a magnet is sufficient to determine suitability for UWMT.
Certification Requirements for UWMT - Personnel performing UWMT require certification in UWMT. Certification can only be obtained by training and examination. Divers may be trained by a certified UWMT examiner. Training can be done at either the divers activity or at the agents facility. Specific Preparation Requirements for UWMT - Preparation for conducting UWMT entails assembling all necessary material and personnel required to safely satisfy the plan requirements. Divers must determine that the water current will not affect the application of magnetic particles where UWMT is to be conducted. Water currents greater than 1 knot makes it difficult to perform UWMT. Divers must also determine that the underwater visibility is adequate for the interpretation of the test results.
- Inspection Equipment Electronic yoke with power cable Ground fault interrupter (GFI) White light source U/W-1 magnetic particles with applicator Magnetic field indicator Surface Preparation and Restoring Equipment Diver staging (optional) Hydraulic or pneumatic hand-held grinder or high-pressure water jet Anti-corrosion coating (epoxy) - Recording Equipment Stereo and/or still camera (optional) Video and monitor system (optional) Measuring devices (tape or rule) Plexiglas writing slate, grease pencil, arrow punch
UWMT equipment includes: Electromagnetic Yoke - An electromagnetic yoke is used to induce a magnetic field in the material. The articulation of the yokes legs allows any pole spacing between 2 inches and 8 inches, and the yoke can accommodate plate offsets of up to 6 inches and joint angles from about 45 degrees to 270 degrees. To minimize the risk of electric shock, no controls are on the yoke. A topside operator energizes the yoke. Power Cable - A two-conductor power cable with a braided external ground and a protective jacket, delivers power to the electromagnetic yoke. Typical cables are 250 feet long to permit operation in the majority of locations accessible by a surface- supported diver. The external ground braid generates a ground fault whenever the cable is cut; the power conductors cannot be reached except by first penetrating the ground braid. Ground Fault Interrupter (GFI) - The divers primary protection from electric shock is an approved isolation transformer/GFI device. The GFI interrupts power when it senses a drop in the resistance between the isolated system power leg and the power supply ground.
White Light Source - A primary illumination source is a Remote Ocean Systems model TUBE-LIGHT. Magnetic Particles - Magnetic particles are finely divided ferromagnetic particles having a low magnetic retentivity and a high permeability. They are dyed pink to be visible under normal lighting. The particles are mixed with wetting agents and corrosion inhibitors to enhance their underwater performance. Magnetic Particle Applicator - The magnetic particle applicator is a reservoir of magnetic particles and water that the diver uses to deliver magnetic particles to the surface of the inspection area. A simple and effective magnetic particle applicator is a plastic squeeze bottle that contains a marble-sized object to aid in mixing. Magnetic Field Indicator - The magnetic field indicator is a small device with cracklike discontinuities on its face. The indicator is used to determine if the inspection site has adequate magnetic flux. The diver places the indicator at the inspection site, topside energizes the yoke, and the diver delivers the particles. A clearly visible accumulation of particles (indications) should then form along the crack-like discontinuities on the pie- shaped magnetic field indicator. In the pie-shaped gauge, the crack-like discontinuities are furnace-brazed joints between adjacent steel wedges. Though a simple test to measure the magnetic field strength inside the material being inspected is unknown, it is assumed that an adequate field just outside the material signifies an adequate field inside as well.
Underwater magnetic particles inspection kit Cracks in a weld